|Year : 2023 | Volume
| Issue : 1 | Page : 85
Effect of hydrogen peroxide and its combination with nano-hydroxyapatite or nano-bioactive glass on the enamel demineralization and tooth color: An in vitro study
Elham Kheradmand1, Alirea Daneshkazemi2, Abdolrahim Davari2, Maede Kave1, Solmaz Ghanbarnejad3
1 Department of Operative Dentistry, Dental Research Center, Dental Research Institute, School of Dentistry, Isfahan University of Medical Sciences, Isfahan, Iran
2 Department of Operative Dentistry, Faculty of Dentistry, Shahid Sadoughi University of Medical Sciences, Yazd, Iran
3 Department of Materials Engineering, Islamic Azad University Tehran Science and Research Branch, Tehran, Iran
|Date of Submission||06-Oct-2021|
|Date of Acceptance||27-Feb-2023|
|Date of Web Publication||25-Jul-2023|
Dr. Elham Kheradmand
Department of Operative Dentistry, Dental Research Center, Dental Research Institute, School of Dentistry, Isfahan University of Medical Sciences, Isfahan
Source of Support: None, Conflict of Interest: None
Background: Patient demand for esthetic dental treatments is increasing, and among different techniques, tooth bleaching is a popular procedure for smile improvement. There is a controversy over the demineralizing effect of hydrogen peroxide (HP) containing bleaching agents on tooth enamel. The aim of this study was to evaluate the effect of HP and its combinations with hydroxyapatite (HA) and bioactive glass (BG) on enamel demineralization and tooth color changes.
Materials and Methods: Three groups of 20 teeth were used. Bleaching regimens included HP alone, HP + HA, and HP + BG. Bleaching was repeated at six periods of 15 min. Energy dispersive spectrometry was performed to evaluate calcium, phosphorus, sodium, magnesium, and fluoride content of superficial enamel before and after bleaching. Tooth color was evaluated by spectrophotometer before and after bleaching and ΔE values were calculated. Data were statistically analyzed using SPSS version 17.
Results: Ca and P content was increased significantly in group HP + BG (P < 0.05). There was no significant difference in ΔE values between the three groups (P > 0.05).(p value = 0.34).
Conclusion: Addition of BG to HP can increase superficial enamel mineral content after bleaching and has no effect on tooth color changes in comparison to HP alone.
Keywords: Bioglass, hydrogen peroxide, hydroxyapatites, tooth bleaching
|How to cite this article:|
Kheradmand E, Daneshkazemi A, Davari A, Kave M, Ghanbarnejad S. Effect of hydrogen peroxide and its combination with nano-hydroxyapatite or nano-bioactive glass on the enamel demineralization and tooth color: An in vitro study. Dent Res J 2023;20:85
|How to cite this URL:|
Kheradmand E, Daneshkazemi A, Davari A, Kave M, Ghanbarnejad S. Effect of hydrogen peroxide and its combination with nano-hydroxyapatite or nano-bioactive glass on the enamel demineralization and tooth color: An in vitro study. Dent Res J [serial online] 2023 [cited 2023 Oct 1];20:85. Available from: https://www.drjjournal.net/text.asp?2023/20/1/85/382138
| Introduction|| |
Discoloration of teeth due to extrinsic or intrinsic origins might compromise the beauty of patient's appearance, increasing the demand for esthetic dental procedures. Among different therapies, tooth bleaching is an easy, cost-effective, and conservative method to enhance tooth appearance.,
The bleaching agents usually contain hydrogen peroxide (HP) or carbamide peroxide (CP) that cause the oxidation of colored organic and inorganic compounds in tooth structure by the decomposition of peroxide into free radicals., However, the reaction is unspecific, and the organic and inorganic materials of the enamel and dentin may be affected, resulting in undesirable topographic effects or mineral loss.
Although studies are controversial on the effect of bleaching on tooth surface's morphological changes, there is a general agreement that peroxide can change tooth mineral content.,,,,
In a few studies, fluoride has been incorporated into bleaching agents to decrease demineralization and expedite the rehardening of enamel., Santos et al. reported the addition of calcium or fluoride to the bleaching gel reduced the erosion effect of HP. Furthermore, some researchers have added nano-HA or nano-bioactive glass (BG) to the bleaching materials to reduce demineralization.,,
Santos et al. found no anti-demineralizing effect by adding nano-HA to HP. However, Khoroushi et al. and Jiang et al. showed that the addition of nano-HA to HP could increase enamel mineral content.
The aim of this study was to describe the effect of HP and its combination with nano-HA or nano-BG on the levels of inorganic elements in enamel and tooth color changes. The null hypothesis was that combining HP with nano-HA or nano-BG had no effects on enamel mineral content or tooth color changes.
| Materials and Methods|| |
This study was developed in accordance with the Code of Ethics in Research (IR.SSU.REC.1396.165). This is an experimental and in vitro study.
Sixty intact and noncarious human premolar teeth extracted for orthodontic reasons were stored in 0.5% chloramine-T solution at 4°C and used within 2 months of extraction.
Teeth were examined by a stereomicroscope (ZTX-20-W, Huaguang, China) at ×20 magnification to exclude any teeth with cracks or structural defects. Teeth were allocated to the three following groups of twenty teeth using random numbers table:
- Group 1 (HP): Bleaching with 40% HP (Boost PF, Ultradent, USA)
- Group 2 (HP + HA): Bleaching with custom gel containing 40% HP (Boost PF) + hydroxyapatite (HA) 2%wt (Sigma-Aldrich, Spain)
- Group 3 (HP + BG): Bleaching with custom gel containing 40% HP (Boost PF) + BG 7.5%wt (NovaBone, Florida, USA).
Final pH of the bleaching agent in each group was measured with pH meter before the application of the material.
After embedding the root in acrylic resin, the buccal surfaces of the tooth crowns were abraded with 600-grit and 1000-grit silicon carbide abrasive papers and subjected to energy dispersive spectrometry (EDS) (Pro-X, Switzerland) analysis to measure Ca, P, Na, Mg, and F contents.
Bleaching procedure was performed following the manufacturer's instructions.
The bleaching agent was applied on the buccal surface of each tooth with a brush for 15 min. Then, the bleaching agent was removed from the surface with a brush, and the samples were rinsed with tap water for 1 min to remove the bleaching gel and were stored in 37°C distilled water until the next bleaching treatment. This was repeated three times in one session for a total of 45 min (3 min × 15 min). The treatment was repeated 1 week later (total six treatments on each tooth). EDS analysis was repeated after the completion of treatment.
Tooth shade was evaluated before and after the bleaching procedure using VITA Easyshade (VITA Zahnfabrik, Germany). L*, a*, and b* parameters were acquired for a reference point 5 mm gingival of the cusp tip three times on each tooth and the mean of the three assessments was used for Δ E calculation.
The data were statistically analyzed using ANOVA, Tukey post hoc, and paired t-test in SPSS software (P < 0.05).(version 17.0, Chicago, IL, USA).
| Results|| |
The pH of the bleaching agents was 5.0 for group HP, 7.0 for group HP + HA, and 9.5 for group HP + BG. Mean and standard deviation of studied elements are presented in [Table 1]. Ca and P content differed significantly between groups after bleaching (ANOVA, P = 0.013 and P = 0.016, respectively), but other studied elements did not show a significant difference. Tukey post hoc showed that both Ca and P contents were significantly higher after bleaching in group HP + BG than group HP + HA (P = 0.014 and P = 0.032, respectively), but groups HP and HP + HA and groups HP and HP + BG did not have a significant difference.
|Table 1: Mean±standard deviation (μg/g) of the studied elements in experiment groups|
Click here to view
Mean Δ E (±standard deviation) was 7.8 ± 2.4 in group HP, 8.1 ± 2.5 in group HP + HA, and 6.8 ± 3.5 in group HP + BG. There was no significant difference between the three study groups.
| Discussion|| |
The aim of this study was to evaluate the effect of HP with or without nano-HA or nano-BG on enamel demineralization and tooth color change. The null hypothesis was that addition of nano-HA and nano-BG to HP did not affect enamel demineralization and tooth color. According to the results, the null hypothesis was rejected.
The use of HP alone did not change the concentration of studied elements. Loss of enamel mineral content following the application of a bleaching agent is controversial. Efeoglu et al. found that office bleaching can reduce the mineral content of enamel extending to a depth of 250 μm. Furthermore, Bizhang et al. concluded that the use of bleaching agents induced mineral loss in bovine tooth enamel. Our study did not confirm these results. A possible explanation may be the inclusion of fluoride compounds (as sodium fluoride) in the bleaching agent, which prevents mineral loss.,,,
Studies about the effect of bleaching on elemental changes are limited. However, some researchers have claimed enamel hardness change is related with its mineral content. Sulieman et al. reported that in vitro use of 35% HP on enamel for 30 min had no effects on enamel or dentin hardness. Faraoni-Romano et al. showed surface microhardness of bovine enamel increased after application of various concentrations of HP and CP. In contrast, Lewinstein et al. and Al-Salehi et al. concluded that enamel microhardness decreases after the use of HP.
Loss of enamel superficial elements has also been investigated in the form of enamel surface roughness changes., Faraoni-Romano et al. reported that the application of different bleaching agents on tooth enamel reduced its surface roughness. McGukin observed a slight increase in enamel surface roughness in his study, but Hunsaker et al. and Gürgan et al. did not seen no surface roughness change. It seems that morphological alterations of enamel are mainly due to the acidity of HP, while decreased microhardness is due to the effect of both demineralization and destruction of organic part by HP.
The different results of studies could be due to different study conditions, including tooth substrates (e.g., human or bovine), bleaching materials, pH, preparation times, procedures (e.g., application of phosphoric acid before bleaching or different specimen storage conditions during experiment),, and discrepancy in performance and measurement methods.
The addition of nano-HA and nano-BG to the bleaching agent increased enamel mineral content in the current study, which is in accordance with Khoroushi et al. and Jiang et al.
Furthermore, Sasaki et al. found the addition of HA to HP increased surface enamel microhardness than samples treated by HP alone. Deng et al. also found similar results using a bleaching agent consisting of HP and BG. Furthermore, it has been shown that application of BG after bleaching caused remineralization by increasing Ca and P values.
Nanoparticle remineralizing materials were used in this study. It has been reported that the use of nano-sized HA increases the remineralization effect because the surface-to-volume ratio increases and the nanoparticles interact with enamel and dentin more effectively. Furthermore, nano-sized BG has been shown to increase dentin remineralization,,, and overcome its long reaction time as an efficient remineralizing material.
The superficial aprismatic enamel is more resistant to demineralization because it is usually hypermineralized and rich in fluorapatite, so we removed this layer and polished it to gain uniform mirror-like surface and minimize the difference among samples.
In the present study, we kept the teeth in distilled water at intervals between bleaching periods. We did not use artificial saliva because it might have a remineralizing effect and interact with HA and BG due to its ionic content.,
All bleaching regimens will be considered effective since a minimum Δ E value of 3.3 is known to be visually comprehensible. Although it is thought that BG deposits may interfere with the penetration of peroxide and whitening efficacy, this speculation was rejected by the current study, which is in accordance with Deng et al., Jiang et al., and Sasaki et al. also found that the addition of HA did not interfere with the whitening results.
Future studies are required to evaluate whether BG or HA application will not decrease bleaching efficacy in vivo.
| Conclusion|| |
Within the limitations of the current study, it can be concluded that fluoride-containing HP bleaching material may not induce loss of superficial enamel mineral content. The addition of nano-HA or nano-BG to the bleaching agent may improve the mineral content (Ca and P) of superficial enamel and will not affect bleaching efficacy.
The authors wish to thank the vice chancellery for research at Yazd university of Medical Sciences for providing financial support for this study with the research project number: 148.
Financial support and sponsorship
Conflicts of interest
The authors of this manuscript declare that they have no conflicts of interest, real or perceived, financial or non-financial in this article.
| References|| |
Khoroushi M, Shirban F, Kaveh S, Doustfateme S. Effect of three nanobiomaterials on microhardness of bleached enamel. Restor Dent Endod 2016;41:196-201.
Alqahtani MQ. Tooth-bleaching procedures and their controversial effects: A literature review. Saudi Dent J 2014;26:33-46.
Sorozini M, Dos Santos RS, Silva EM, Dos Anjos MJ, Perez CR. Assessment of Ca and P content variation in enamel during an eight-week bleaching protocol using energy dispersive X-ray fluorescence. Spectrochim Acta Part B At Spectrosc 2017;131 Suppl C: 93-8.
Zuryati AG, Qian OQ, Dasmawati M. Effects of home bleaching on surface hardness and surface roughness of an experimental nanocomposite. J Conserv Dent 2013;16:356-61.
] [Full text]
Rastelli AN, Nicolodelli G, Romano RA, Milori DM, Perazzoli IL, Ferreira EJ, et al.
After bleaching enamel remineralization using a bioactive glass-ceramic (BioSilicate®
). Biomed Glasses 2016;2:1-9.
Ben-Amar A, Liberman R, Gorfil C, Bernstein Y. Effect of mouthguard bleaching on enamel surface. Am J Dent 1995;8:29-32.
Ernst CP, Marroquín BB, Willershausen-Zönnchen B. Effects of hydrogen peroxide-containing bleaching agents on the morphology of human enamel. Quintessence Int 1996;27:53-6.
Haywood VB, Heymann HO. Nightguard vital bleaching: How safe is it? Quintessence Int 1991;22:515-23.
Al-Salehi SK, Wood DJ, Hatton PV. The effect of 24h non-stop hydrogen peroxide concentration on bovine enamel and dentine mineral content and microhardness. J Dent 2007;35:845-50.
Attin T, Schmidlin PR, Wegehaupt F, Wiegand A. Influence of study design on the impact of bleaching agents on dental enamel microhardness: A review. Dent Mater 2009;25:143-57.
Deng M, Wen HL, Dong XL, Li F, Xu X, Li H, et al.
Effects of 45S5 bioglass on surface properties of dental enamel subjected to 35% hydrogen peroxide. Int J Oral Sci 2013;5:103-10.
Santos LF, Torres CR, Caneppele TM, Magalhães AC, Borges AB. Effect of home-bleaching gels modified by calcium and/or fluoride and the application of nano-hydroxyapatite paste on in vitro
enamel erosion susceptibility. Acta Odontol Scand 2016;74:121-6.
Pedreira De Freitas AC, Botta SB, Teixeira Fde S, Salvadori MC, Garone-Netto N. Effects of fluoride or nanohydroxiapatite on roughness and gloss of bleached teeth. Microsc Res Tech 2011;74:1069-75.
Gjorgievska E, Nicholson JW. Prevention of enamel demineralization after tooth bleaching by bioactive glass incorporated into toothpaste. Aust Dent J 2011;56:193-200.
Jiang T, Ma X, Wang Z, Tong H, Hu J, Wang Y. Beneficial effects of hydroxyapatite on enamel subjected to 30% hydrogen peroxide. J Dent 2008;36:907-14.
Godinho J, Silveira J, Mata A, Carvalho ML, Pessanha S. Effect of bleaching gel in Ca, P and Zn content in tooth enamel evaluated by μ-EDXRF. Nucl Instrum Methods Phys Res B 2014;337:78-82.
Miranda CB, Pagani C, Benetti AR, Matuda Fda S. Evaluation of the bleached human enamel by scanning electron microscopy. J Appl Oral Sci 2005;13:204-11.
Sakaguchi RL, Ferracane JL, Powers JM. Craig's restorative dental materials. 14th
ed. St. Louis (Missouri): Elsevier, Cop; 2019.
Efeoglu N, Wood DJ, Efeoglu C. Thirty-five percent carbamide peroxide application causes in vitro
demineralization of enamel. Dent Mater 2007;23:900-4.
Bizhang M, Seemann R, Duve G, Römhild G, Altenburger JM, Jahn KR, et al.
Demineralization effects of 2 bleaching procedures on enamel surfaces with and without post-treatment fluoride application. Oper Dent 2006;31:705-9.
Faraoni-Romano JJ, Da Silveira AG, Turssi CP, Serra MC. Bleaching agents with varying concentrations of carbamide and/or hydrogen peroxides: Effect on dental microhardness and roughness. J Esthet Restor Dent 2008;20:395-402.
Attin T, Betke H, Schippan F, Wiegand A. Potential of fluoridated carbamide peroxide gels to support post-bleaching enamel re-hardening. J Dent 2007;35:755-9.
Gladwell J, Simmons D, Wright JT. Remineralization potential of a fluoridated carbamide peroxide whitening gel. J Esthet Restor Dent 2006;18:206-12.
Tanizawa Y. Reaction characteristics of a tooth-bleaching agent containing H2O2 and NaF: In vitro
study of crystal structure change in treated hydroxyapatite and chemical states of incorporated fluorine. J Cosmet Sci 2005;56:121-34.
Sulieman M, Addy M, Macdonald E, Rees JS. A safety study in vitro
for the effects of an in-office bleaching system on the integrity of enamel and dentine. J Dent 2004;32:581-90.
Lewinstein I, Fuhrer N, Churaru N, Cardash H. Effect of different peroxide bleaching regimens and subsequent fluoridation on the hardness of human enamel and dentin. J Prosthet Dent 2004;92:337-42.
Ulukapi H. Effect of different bleaching techniques on enamel surface microhardness. Quintessence Int 2007;38:e201-5.
Attin T, Müller T, Patyk A, Lennon AM. Influence of different bleaching systems on fracture toughness and hardness of enamel. Oper Dent 2004;29:188-95.
Sasaki RT, Catelan A, Bertoldo Edos S, Venâncio PC, Groppo FC, Ambrosano GM, et al.
Effect of 7.5% hydrogen peroxide containing remineralizing agents on hardness, color change, roughness and micromorphology of human enamel. Am J Dent 2015;28:261-7.
Generosi A, Rau JV, Rossi Albertini V, Paci B. Crystallization process of carbonate substituted hydroxyapatite nanoparticles in toothpastes upon physiological conditions: An in situ
time-resolved X-ray diffraction study. J Mater Sci Mater Med 2010;21:445-50.
Curtis AR, West NX, Su B. Synthesis of nanobioglass and formation of apatite rods to occlude exposed dentine tubules and eliminate hypersensitivity. Acta Biomater 2010;6:3740-6.
Vollenweider M, Brunner TJ, Knecht S, Grass RN, Zehnder M, Imfeld T, et al.
Remineralization of human dentin using ultrafine bioactive glass particles. Acta Biomater 2007;3:936-43.
Lee BS, Tsai HY, Tsai YL, Lan WH, Lin CP. In vitro
study of DP-bioglass paste for treatment of dentin hypersensitivity. Dent Mater J 2005;24:562-9.
Bakry AS, Takahashi H, Otsuki M, Sadr A, Yamashita K, Tagami J. CO2 laser improves 45S5 bioglass interaction with dentin. J Dent Res 2011;90:246-50.
Kanemura N, Sano H, Tagami J. Tensile bond strength to and SEM evaluation of ground and intact enamel surfaces. J Dent 1999;27:523-30.